PHYSICAL REVIEW B 75, 033316 2007

**Zero** g **factors** **and** **nonzero** **orbital** **momenta** **in** **self**-**assembled** quantum dots

Weidong Sheng

Department of Physics, Fudan University, Shanghai 200433, Ch**in**a

**and** Institute for Microstructural Sciences, National Research Council, Ottawa, Ontario, Canada K1A 0R6

A. Bab**in**ski

Institute of Experimental Physics, Warsaw University, Hoza 69, 00-681 Warszawa, Pol**and**

Received 8 December 2006; published 26 January 2007

We po**in**t out us**in**g an empirical tight-b**in**d**in**g approach that the ground state of holes **in** InAs/GaAs

**self**-**assembled** quantum dots carries **nonzero** **orbital** momentum. The sp**in** **and** **orbital** motions of the hole state

are found to have opposite contributions to the hole g factor, lead**in**g to zero g **factors** of holes **and** then

excitons **in** dots of high aspect ratio. The **nonzero** envelope **orbital** **momenta** of the holes are also shown to

account for anisotropic circular polarization of exciton emission **and** nonl**in**ear Zeeman splitt**in**gs **in** high

magnetic fields. Our theory well expla**in**s recent experiments **and** **in**dicates the possibility of eng**in**eer**in**g

magnetic splitt**in**g by tun**in**g the electric conf**in**ement **in** nanostructures.

DOI: 10.1103/PhysRevB.75.033316

PACS numbers: 71.18.y, 78.67.Hc, 73.21.La

As one of the most important magnetic properties of a

system, the g factor measures the Zeeman splitt**in**g of an

electron state **in** a magnetic field **and** is determ**in**ed by both

the sp**in** **and** **orbital** motion of the electron. In semiconductors

like InAs **and** GaAs, the **orbital** motion of localized p

**orbital**s is strongly coupled to the sp**in**, **and** the result**in**g

valence-b**and** states can be classified by the correspond**in**g

total angular momentum. Heavy **and** light holes, identified

by their different angular **momenta**, have dist**in**ctive g **factors**,

i.e., g hh =−6 **and** g s lh =−2 where is an empirical

s

parameter **in** the k· p theory. 1

In addition to the **orbital** motion of localized atomic **orbital**s,

electrons **in** nanostructures like **self**-**assembled** quantum

dots 2 can also acquire **orbital** magnetic moment due to

the motion around the circumference of the structures. However,

it is often taken for granted that the ground state of a

s**in**gle exciton **in** these artificial atoms does not carry any

**nonzero** **orbital** **momenta** largely because the lowest level of

a natural atom is known to always have zero **orbital** momentum.

Such ignorance of the **orbital** motion can greatly impede

the underst**and****in**g of electron **and** hole g **factors** **in**

quantum dots. 3

While it is true that the ground state of electrons **in** quantum

dots does not carry any angular momentum, we f**in**d that

the ground state of holes does carry **nonzero** envelope angular

**momenta**. In the present work, we will show that the

**nonzero** envelope **orbital** **momenta** NEOM of holes is essential

to underst**and** the behavior of g **factors** of holes **and**

excitons **and** can expla**in** the zero exciton g factor **and** nonl**in**ear

Zeeman splitt**in**gs observed **in** a recent experiment.

Moreover, we predict that the NEOM would lead to anisotropic

circular polarization of the exciton emission.

For the purpose of this study, we choose an sp 3 tightb**in**d**in**g

method 4 which has been successfully applied **in** ferromagnetic

quantum wells. 5 The one-electron tight-b**in**d**in**g

Hamiltonian describes an electron hopp**in**g from atomic sp**in**

**orbital** , at position R to sp**in** **orbital** , at position

R:

H tb =

†

where c R,,

R,,,R,,

†

HR,,;R,,c R,, c R ,,,

1

c R ,, are creation annihilation operators.

The basis of the sp**in** **orbital**s is chosen as

s ↓ ,x ↓ ,y ↓ ,z ↓ ,s ↑ ,x ↑ ,y ↑ ,z ↑ . The hopp**in**g matrix

elements **and** site energies for s **and** p **orbital**s are extended

to **in**clude second-nearest-neighbor **in**teractions 6 to fit the effective

masses of electrons **and** holes at the po**in**t **and**

conduction- **and** valence-b**and** edges at both the **and** X

po**in**ts exactly. Sp**in**-orbit **in**teraction is also **in**corporated.

In a magnetic field, Peierls phase **factors** are **in**troduced to

transform the off-diagonal matrix elements as

HR,R → exp− i e R

Ardr HR,R, 2

R

where Ar is the vector potential. The Zeeman effect is

**in**cluded by add**in**g the sp**in** terms to the diagonal matrix

elements,

HR ↑↓ ,R ↑↓ → HR ↑↓ ,R ↑↓ ± 1 2 g BB z ,

where g is the g factor of a bare electron. It is noted that no

additional empirical parameters like are used for the Zeeman

effect.

The calculations of electron **and** hole g **factors** are performed

for a typical lens-shaped InAs/GaAs quantum dot

which is 20 nm long **in** diameter, on a 2 monolayer wett**in**g

layer **and** has a vary**in**g height. The total number of atoms

**in**cluded **in** the calculation is about 500 000. A Lanczos algorithm

is used to compute the eigenvalues **and** eigenvectors

of large sparse matrices generated by the tight-b**in**d**in**g

Hamiltonian. The calculation is first performed for the stra**in**

distribution by an atomistic valence-force-field method, followed

by an analysis of the electronic structure by the tightb**in**d**in**g

method.

3

1098-0121/2007/753/0333164

033316-1

©2007 The American Physical Society

BRIEF REPORTS

PHYSICAL REVIEW B 75, 033316 2007

FIG. 1. Color onl**in**e The L**and**é g **factors** of holes **and** electrons,

calculated as a function of the height of the lens-shaped **self****assembled**

InAs/GaAs quantum dots as shown **in** the **in**set. The

heights of the dots are **in** units of the lattice constant of GaAs.

Figure 1 plots the calculated hole **and** electron g **factors**,

g h **and** g e , as a function of the height of the dots. The result

exhibits a weak dependence of the electron g factor on the

height of the dots H. However, the hole g factor is found to

**in**crease rapidly as the height H becomes larger. The comb**in**ed

exciton g factor, g ex =g h +g e , is seen to change from

−1.47 when H3.4 nm to 0.09 when H6.2 nm. Hence,

the exciton g factor vanishes at a po**in**t between 10a **and** 11a.

In a recent magnetospectroscopy experiment of on s**in**gle

InAs/GaAs quantum dots, 7 the exciton g **factors** of two

s**in**gle dots were measured; one was about 3 nm high **and**

had g ex =−1.5 **and** the other was about 5 nm high **and** had an

almost zero exciton g factor, which nearly quantitatively

agrees with our theoretical calculation.

In the follow**in**g, we will expla**in** why the g factor of holes

**and** then excitons would vanish as the height of the dots

**in**creases. Let us start with an analysis of valence-b**and** states

**in** **self**-**assembled** quantum dots. Because of the **in**fluence of

the b**and** mix**in**g **and** stra**in** field, the valence-b**and** states **in**

quantum dots are much more complex than those **in** the conduction

b**and**s. In general, a hole state **in** quantum dots is

composed of components from the heavy hh, light lh, **and**

split-off sh hole b**and**s, **and** the conduction b**and**s s. Itcan

be written as = n n↑ n ↑ + n↓ n ↓ , where n

=hh,lh,sh,s. 8–10 If only the contribution from the Bloch

functions is taken **in**to account, the hole g factor can then be

expressed as g s h = n g n c n↑ −c n↓ , where g n is the g factor for

b**and** n **and** c n = n n 2 . 11 Consider**in**g that the ground

state of the holes is dom**in**ated by its heavy **and** light hole

components, we have g s h g s hh c hh↑ +g s lh c lh↑ . It gives us a

simple theory to expla**in** why the hole g factor becomes

smaller when the proportion of the heavy hole component

decreases, 12 which has been quite successful **in** quantum

wells where the lateral motion of carriers is not conf**in**ed.

However, **in** quantum dots with strong lateral conf**in**ement,

underst**and****in**g of the hole g factor would nevertheless require

knowledge of the spatial distribution of the envelope functions

of both heavy **and** light hole components.

Figure 2 plots the probability density of the light lh↑ 2

**and** heavy hh↑ 2 hole components **in** the ground state of

the holes **in** a dot of H=6a. The expectation value of the

FIG. 2. Color onl**in**e Plots of light **and** heavy hole envelope

functions **in** the ground state of holes **in** a flat lens-shaped

InAs/GaAs quantum dot. The expectation values of the **orbital** momentum

operator L z are labeled.

**orbital** momentum operator **in** the envelope functions of the

light **and** heavy hole components can be calculated by Lˆ z

= h x/y−y/x h . Similar to the ground state of

the electrons, we f**in**d that the **orbital** momentum of the

dom**in**ant heavy hole component is very small L z 0.01.

However, the light hole components are found to carry **nonzero**

angular **momenta**, i.e., L z =0.99 for lh↑ **and** L z

=1.79 for lh↓ .

The reason why the heavy hole component of zero angular

momentum mixes with the light hole parts of **nonzero**

angular **momenta** lies **in** the fact that the total angular momentum,

i.e., the envelope part plus the Bloch part L z + j z ,

is a good quantum number **in** a system with cyl**in**drical

symmetry. 8,9,13,14 Even if the symmetry is broken by the

shear stra**in**, we f**in**d that the conservation of the total angular

momentum is still a good approximation.

Includ**in**g the contribution from the envelope functions,

we have the overall hole g factor

g h = g h s + g h o ,

where g h o denotes the contribution from NEOM,

g o h =2 n↑ Lˆ zn↑

+ n↓ Lˆ zn↓

. 5

n

In the dot of flat shape as shown **in** Fig. 2, the light hole

components have a very small projection **in** the ground state

of holes, i.e., c lh↑ =1.86% **and** c lh↓ =0.41%; hence NEOM

give only a small contribution to the hole g factor. As the

light hole components take a larger proportion, the contribution

from the envelope part becomes more important to the

hole g factor.

Figure 3 plots the envelope **orbital** **momenta** of the heavy

**and** light hole components, i.e., hh↑ Lˆ zhh↑

/c hh↑ **and**

hh↑ Lˆ zlh↑

/c lh↑ , **and** g o h , as a function of the height of

dots. As the aspect ratio of the dot **in**creases, the light hole

component is found to have a larger projection c lh↑ +c lh↓ **in**

the ground state of holes due to its stronger mixture with the

4

033316-2

BRIEF REPORTS

PHYSICAL REVIEW B 75, 033316 2007

FIG. 3. Envelope **orbital** **momenta** of the heavy **and** light hole

components **in** the ground state of holes **and** the correspond**in**g

equivalent g factor calculated as a function of the height of the

lens-shaped **self**-**assembled** InAs/GaAs quantum dot as shown **in**

the **in**set of Fig. 1.

heavy hole part. 12 For example, when the height of the dot

H changes from 6a3.4 nm to 11a6.2 nm where a is

the lattice constant of GaAs, c lh↑ +c lh↓ **in**creases from 2.0%

to 7.1%; **in** the meantime, the proportion of the heavy hole

part c hh↑ +c hh↓ drops from 96.6% to 89.0%.

Correspond**in**g to these changes, the equivalent g factor

due to NEOM, g h o , becomes larger. Moreover, the heavy hole

component starts to ga**in** noticeable NEOM when H8a,

which gives a significant contribution to g h o . For example, the

contribution from the heavy hole part alone accounts for

41% of g h o when H=9a while it **in**creases to 61% when H

=11a. When the dot is flat, we f**in**d that the contribution from

NEOM g h o is small **and** the hole g factor is dom**in**ated by

that from the Bloch parts g h s . In this case, we have

g h o ≪g h s while g h s 0 **and** g h o 0. With the **in**crease of the

aspect ratio of the dot, g h o becomes larger because of not only

the larger proportion of the light hole component but also the

NEOM of the heavy hole parts.

As the aspect ratio of the dot **in**creases, the contribution

from the Bloch parts g h s is seen to become smaller while

that from the envelope **orbital** **momenta** g h o becomes the

dom**in**ant part **in** the hole g factor. Because the two parts g h

s

**and** g h o have the opposite signs, they are found to nearly

cancel each other when H=10a, which results **in** an almost

zero hole g factor. When the aspect ratio **in**creases further,

g h o becomes larger than g h s , which leads to the change of

the sign of the overall hole g factor. At H=11a, the hole g

factor is found to become positive **and** nearly cancel the electron

g factor, lead**in**g to an almost zero exciton g factor,

which well expla**in**s the zero exciton g factor observed **in** the

recent experiment. 7

While the result shown **in** Fig. 2 may also be obta**in**ed by

the eight-b**and** k· p method, 15 we f**in**d that it is necessary to

apply the tight-b**in**d**in**g approach for the calculation of the g

**factors**. The key to this issue is that the parameter used **in**

the k· p theory is not well established. Even **in** quantum

wells, a fitt**in**g procedure is often required to reproduce the

experimental data, 16 **and** xxx the uncerta**in**ty **in** its value can

be as large as 10%. In our k· p calculation, a mere 3% change

**in** from 7.68 to 7.48 can **in**duce a change of more than

FIG. 4. Color onl**in**e The proportion of the heavy hole component

**in** the sp**in**-up **and** sp**in**-down states of the holes **and** the circular

polarization of the exciton emission, calculated as a function of

magnetic field **in** a lens-shaped InAs/GaAs quantum dot.

20% **in** the result**in**g hole g factor from 0.30 to 0.24. Another

difficulty we encounter **in** the k· p calculation is that **in**

most cases it gives electron **and** hole g **factors** with opposite

signs, 12 which is **in** an obvious contradiction with the experiment

where the electron **and** hole g **factors** are shown to have

the same sign. 3

Besides the zero g **factors** of holes **and** excitons, the **in**terplay

between the contributions from the Bloch **and** envelope

parts g h **and** g o h can lead to many other observable

s

effects such as anisotropic circular polarization of the exciton

emission **in** a high magnetic field. Let us take the example of

the dot with height H=10a. As can be seen **in** Fig. 1, the

overall hole g factor nearly vanishes due to the opposite

contribution from the heavy **and** light hole parts. It can be

estimated that the effective g factor **in**clud**in**g both the

Bloch parts **and** NEOM for the heavy hole part is g hh

−0.07 **and** for the light hole part g lh 0.08. As the magnetic

field **in**creases, the heavy hole part of the sp**in**-up state tends

to lower its energy because g hh 0. In the meantime, its light

hole part tends to do the opposite s**in**ce g lh 0. The competition

means that the sp**in**-up state ga**in**s more heavy hole part

while los**in**g the light hole part as the field **in**creases. A similar

process also goes on **in** the sp**in**-down state, but, end**in**g

with the opposite dependence.

The calculated c hh↑ **and** c hh↓ are plotted as a function of

the magnetic field **in** Fig. 4, **and** exhibit the predicted dependence.

As the **in**tensity of the + − transition is ma**in**ly

determ**in**ed by the proportion of the heavy hole components

**in** the sp**in**-up sp**in**-down hole state, the polarized heavy

hole components directly lead to the anisotropic circular polarization

of the exciton emission. The calculated degree of

circular polarization def**in**ed 17 by p=I +−I −/I ++I − is

plotted **in** Fig. 4, **and** is seen to **in**crease with the magnetic

field. It is noted that due to the sp**in** relaxation effect, this

phenomenon may not be well resolved when l**in**early polarized

excitation is applied. Instead, circularly polarized excitation

should be used for the observation of this effect.

Another observable phenomenon **in**duced by NEOM is

nonl**in**ear Zeeman splitt**in**gs. As the sp**in**-down state is noticed

to lose its heavy hole component faster than the sp**in**-up

state ga**in**s the heavy hole component, the total projection of

the heavy hole components **in** the sp**in**-up **and** sp**in**-down

033316-3

BRIEF REPORTS

hole states decreases as the magnetic field **in**creases, which

causes the g factor of holes to change as the magnetic field

**in**creases **and** leads to weak yet observable nonl**in**ear Zeeman

splitt**in**gs. 7

NEOM also exist **in** other k**in**ds of systems like carbon

nanotubes. 18 Although the motion of carriers is not conf**in**ed

**in** the lateral directions **in** quantum wells, a magnetic field

applied along the growth direction would **in**duce lateral **orbital**

motion that mixes heavy **and** light hole states. Such a

b**and** mixture sometimes leads to strong nonl**in**ear Zeeman

splitt**in**g. 16 In spite of some similarities between the **orbital**

motion **in** quantum dots discussed here **and** that **in**duced by

the applied magnetic field **in** quantum wells, the difference is

obvious: NEOM **in** **self**-**assembled** quantum dots are **in**duced

by the structural conf**in**ement **and** hence represent an **in**tr**in**sic

property that does not depend on an external field. While

it may be argued that the mechanism lead**in**g to NEOM has

been **in**cluded **in** previous work, 12 we would like to rem**in**d

the reader that NEOM have not been explicitly studied, let

alone their effect on the g factor of holes **in** quantum dots.

On the contrary, it has recently been reported that the behavior

of the hole g factor **in** quantum dots can be understood **in**

PHYSICAL REVIEW B 75, 033316 2007

terms of **orbital** momentum quench**in**g, 19 which is proved

**in**correct by our calculation.

As a result of NEOM, the light hole component **in** the

ground state of holes has almost zero overlap with the

ground state of electrons **in** a flat quantum dot; therefore, it

has little contribution to the **in**terb**and** transition. As the aspect

ratio **in**creases, L z = lh L z lh − e L z e starts to

deviate from 1, which partially lifts the forbidden transition.

In conclusion, we f**in**d that the hole g factor has two dist**in**ct

contributions **in** **self**-**assembled** quantum dots, one from

the Bloch functions **and** the other from the **nonzero** **orbital**

**momenta** carried **in** the envelope functions of the holes. We

show that these two contributions to the hole g factor have

opposite signs **and** account for the zero g **factors** of holes **and**

excitons **in** dots of high aspect ratio. We also po**in**t out that

the **nonzero** **orbital** **momenta** are responsible for anisotropic

circular polarization of the exciton emission **and** nonl**in**ear

Zeeman splitt**in**gs.

This work is supported by the NSFC Nos. 10644001 **and**

10634040. The authors thank P. Hawrylak **and** M. Korkus**in**ski

for discussions.

1 M. H. Weiler, **in** Semiconductors **and** Semimetals, edited by R. K.

Willardson **and** A. C. Beer Academic, New York, 1981, Vol.

16, p. 119.

2 D. Bimberg, M. Grundmann, **and** N. N. Ledentsov, Quantum Dot

Heterostructures Wiley, New York, 1999.

3 M. Bayer, A. Kuther, A. Forchel, A. Gorbunov, V. B. Timofeev,

F. Schäfer, J. P. Reithmaier, T. L. Re**in**ecke, **and** S. N. Walck,

Phys. Rev. Lett. 82, 1748 1999; M. Bayer, A. Kuther, F.

Schäfer, J. P. Reithmaier, **and** A. Forchel, Phys. Rev. B 60,

R8481 1999.

4 S. J. Sun **and** Y.-C. Chang, Phys. Rev. B 62, 13631 2000.

5 I. Vurgaftman **and** J. R. Meyer, Phys. Rev. B 64, 245207 2001.

6 W. Sheng **and** P. Hawrylak, Phys. Rev. B 73, 125331 2006.

7 A. Bab**in**ski, G. Ortner, S. Raymond, M. Potemski, M. Bayer, W.

Sheng, P. Hawrylak, Z. Wasilewski, S. Fafard, **and** A. Forchel,

Phys. Rev. B 74, 075310 2006.

8 O. Stier, Ph.D. thesis, Berl**in** Studies **in** Solid State Physics Vol. 7

W&T, Berl**in**, 2000.

9 M. Grundmann, Nano-Optoelectronic: Concepts, Physics **and** Devices

Spr**in**ger, Berl**in**, 2002.

10 W. Sheng, S.-J. Cheng, **and** P. Hawrylak, Phys. Rev. B 71,

035316 2005.

11 A. V. Nenashev, A. V. Dvurechenskii, **and** A. F. Z**in**ovieva, Phys.

Rev. B 67, 205301 2003.

12 T. Nakaoka, T. Saito, J. Tatebayashi, **and** Y. Arakawa, Phys. Rev.

B 70, 235337 2004; T. Nakaoka, T. Saito, J. Tatebayashi, S.

Hirose, T. Usuki, N. Yokoyama, **and** Y. Arakawa, ibid. 71,

205301 2005.

13 U. Woggon, Optical Properties of Semiconductor Quantum Dots,

Spr**in**ger Tracts **in** Modern Physics Vol. 136 Spr**in**ger, Berl**in**,

1996.

14 L. G. C. Rego, P. Hawrylak, J. A. Brum, **and** A. Wojs, Phys. Rev.

B 55, 15694 1997.

15 W. Sheng **and** J.-P. Leburton, Phys. Status Solidi B 237, 394

2003.

16 N. J. Traynor, R. T. Harley, **and** R. J. Warburton, Phys. Rev. B 51,

7361 1995; N. J. Traynor, R. J. Warburton, M. J. Snell**in**g, **and**

R. T. Harley, ibid. 55, 15701 1997.

17 A. Kuther, M. Bayer, A. Forchel, A. Gorbunov, V. B. Timofeev,

F. Schäfer, **and** J. P. Reithmaier, Phys. Rev. B 58, R7508 1998.

18 E. D. M**in**ot, Yuval Yaish, V. Sazonova, **and** P. L. McEuen, Nature

London 428, 536 2004.

19 C. E. Pryor **and** M. E. Flatté, Phys. Rev. Lett. 96, 026804 2006.

033316-4